Ion release, antimicrobial and physio-mechanical properties of glass ionomer cement containing micro or nanosized hexametaphosphate, and their effect on enamel demineralization
- 77 Downloads
To evaluate the effects of hexametaphosphate microparticles (mHMP) or nanoparticles (nHMP) incorporated in glass ionomer cement (GIC) on antimicrobial and physico-mechanical properties, fluoride (F) release, and enamel demineralization.
Material and methods
HMP solutions were obtained at concentrations of 1, 3, 6, 9, and 12%, for screening of antimicrobial activity. Next, mHMP or nHMP at 6, 9, and 12% were incorporated into a resin-modified GIC and the antibacterial activity was evaluated. The resistance to diametral tensile and compressive strength, surface hardness, and degree of monomer conversion as well as F and HMP releases of GICs were determined. Furthermore, specimens were attached to enamel blocks and submitted to pH-cycling, and mineral loss was determined. Parametric and non-parametric tests were performed, after checking data homoscedasticity (p < 0.05).
HMP solutions at 6, 9, and 12% demonstrated the best antibacterial activity. GIC containing HMP showed better antibacterial effects at 9 and 12% for nHMP. Regarding F and HMP releases, the highest levels of release occurred for groups containing 9 and 12% nHMP. With the increase in HMP concentration, there was lower mineral loss. However, the incorporation of mHMP or nHMP in GIC reduced values of physico-mechanical properties when compared to the control GIC.
nHMP improves antimicrobial activity and fluoride release, and decreases enamel demineralization, but reduces the physico-mechanical properties of GIC.
The association of GIC/HMP could be an alternative material for patients at high risk for dental caries and could be indicated for low-stress regions or provisional restorations.
KeywordsGlass ionomer cements Phosphates Nanoparticles Polymerization Compressive strength Antibacterial agents
The authors acknowledge the financial support of the scholarship provided by the National Council of Technological and Scientific Development (CNPq 134267/2014-1) and wish to thank Dr. Emerson Rodrigues Camargo for his help in the synthesis of nanosized HMP.
The study was supported by the scholarship provided by the National Council of Technological and Scientific Development (CNPq 134267/2014-1).
Compliance with ethical standards
Conflict of interest
The authors declare that they have no conflict of interest.
This article does not contain any studies with human participants or animals performed by any of the authors.
This article does not contain any studies with human participants performed by any of the authors.
- 6.Khoroushi M, Keshani F (2013) A review of glass-ionomers: from conventional glass-ionomer to bioactive glass-ionomer. Dent Res J (Isfahan) 10(4):411–420Google Scholar
- 14.de Castilho AR, Duque C, Negrini TC, Sacono NT, de Paula AB, de Souza Costa CA, Spolidório DM, Puppin-Rontani RM (2013) In vitro and in vivo investigation of the biological and mechanical behaviour of resin-modified glass-ionomer cement containing chlorhexidine. J Dent 41:155–163. https://doi.org/10.1016/j.jdent.2012.10.014 CrossRefPubMedGoogle Scholar
- 18.Hook ER, Owen OJ, Bellis CA, Holder JA, O’Sullivan DJ, Barbour ME (2014) Development of a novel antimicrobial-releasing glass ionomer cement functionalized with chlorhexidine hexametaphosphate nanoparticle. J Nanobiotechnology 12:3. 17. https://doi.org/10.1186/1477-3155-12-3 CrossRefPubMedPubMedCentralGoogle Scholar
- 19.Bellis CA, Nobbs AH, O'Sullivan DJ, Holder JA, Barbour ME (2016) Glass ionomer cements functionalised with a concentrated paste of chlorhexidine hexametaphosphate provides dose-dependent chlorhexidine release over at least 14 months. J Dent 45:53–58. https://doi.org/10.1016/j.jdent.2015.12.009 CrossRefPubMedGoogle Scholar
- 22.Fiske CH, Subbarow Y (1925) The colorimetric determination of phosphorus. J Biol Chem 66:375–400 - 21Google Scholar
- 30.Forss H, Jokinen J, Spets-Happonen S, Seppa L, Luoma H (1991) Fluoride and mutans streptococci in plaque grown on glass-ionomer and composite. Caries Res 25(454–458):26Google Scholar
- 33.van Dijk JW, Borggreven JM, Driessens FC (1980) The effect of some phosphates and a phosphonate on the electrochemical properties of bovine enamel. Arch Oral Biol 25:591–595Google Scholar
- 34.De Gee AJ (1999) Physical properties of glass-ionomer cements: setting shrinkage and wear. In: Davidson CL, Mjor IA (ed) Advances in glass-ionomer cements. Quintessence, Illinois, pp51–65 -29Google Scholar
- 39.Khouw-Liu VH, Anstice HM, Pearson GJ (1999) An in vitro investigation of a poly (vinyl phosphonic acid) based cement with four conventional glass-ionomer cements. Part 1: Flexural strength and fluoride release. J Dent 27:351–357-28. https://doi.org/10.1016/S0300-5712(98)00062-1 CrossRefGoogle Scholar
- 41.Dancey CP, Reidy J (2011) Statistics without maths for psychology. 5th edn. Pearson, London 620p. 35Google Scholar
- 42.Soh MS, Yap AU, Siow KS (2003) The effectiveness of cure of LED and halogen curing lights at varying cavity depths. Oper Dent 28(707–715):36Google Scholar